Table 19. Continued. 













Corrosion 







Alloy 



CDA 



No. a 



Environment 



Exposure 

 (day) 



Depth 



(ft) 



Rate 



(mpy) 



Type of 

 Corrosion* 7 



Source 



Si Bronze A 



655 



W 



1,064 



5,300 



0.6 



SL-CO 



INCO (3) 



Si Bronze A 



655 



S 



1,064 



5,300 



0.4 



U 



INCO (3) 



Si Bronze A 



655 



w 



197 



2,340 



0.8 



U 



Boeing (6) 



Si Bronze A 



655 



w 



197 



2,340 



0.9 



U 



CEL (4) 



Si Bronze A 



655 



w 



197 



2,340 



1.1 



U 



INCO (3) 



Si Bronze A 



655 



S 



197 



2,340 



0.6 



U 



CEL (4) 



Si Bronze A 



655 



S 



197 



2,340 



0.2 



U 



INCO (3) 



Si Bronze A 



655 



w 



402 



2,370 



1.0 



ET 



CEL (4) 



Si Bronze A 



655 



w 



402 



2,370 



0.8 



U 



INCO (3) 



Si Bronze A 



655 



S 



402 



2,370 



0.8 



ET 



CEL (4) 



Si Bronze A 



655 



s 



402 



2,370 



0.1 



ET 



INCO (3) 



Si Bronze A 



655 



w 



181 



5 



1.8 



U 



CEL (4) 



Si Bronze A 



655 



w 



181 



5 



1.6 



G 



INCO (3) 



Si Bronze A 



655 



w 



366 



5 



1.2 



G 



INCO (3) 



Si Bronze A 



655 



w 



398 



5 



1.1 



G 



CEL (4) 



Si Bronze A 



655 



w 



540 



5 



2.5 



CR(30);C(15) 



CEL (4) 



Si Bronze A 



655 



w 



588 



5 



0.9 



CR(9) 



CEL (4) 



Ni-Vee Bronze A 



- 



w 



123 



5,640 



0.7 



U 



INCO (3) 



Ni-Vee Bronze A 



- 



s 



123 



5,640 



0.5 



U 



INCO (3) 



Ni-Vee Bronze A 



- 



w 



403 



6,780 



0.6 



U 



INCO (3) 



Ni-Vee Bronze A 



- 



s 



403 



6,780 



0.3 



U 



INCO (3) 



Ni-Vee Bronze A 



- 



w 



751 



5,640 



2.6 



s ! 



INCO (3) 



Ni-Vee Bronze A 



- 



s 



751 



5,640 



0.4 



u 



INCO (3) 



Ni-Vee Bronze A 



- 



w 



1,064 



5,300 



2.2 



CR (20) 



INCO (3) 



Ni-Vee Bronze A 



- 



s 



1,064 



5,300 



0.3 



u 



INCO (3) 



Ni-Vee Bronze A 



- 



w 



197 



2,340 



0.6 



u 



INCO (3) 



Ni-Vee Bronze A 



- 



s 



197 



2,340 



<0.1 



NU-ET 



INCO (3) 



Ni-Vee Bronze A 



- 



w 



402 



2,370 



0.4 



U 



INCO (3) 



Ni-Vee Bronze A 



- 



s 



402 



2,370 



<0.1 



ET 



INCO (3) 



Ni-Vee Bronze A 



- 



w 



181 



5 



2.0 



P(7) 



INCO (3) 



Ni-Vee Bronze A 



- 



w 



366 



5 



1.5 



CR(10) 



INCO (3) 



Ni-Vee Bronze B 



- 



w 



123 



5,640 



0.6 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



s 



123 



5,640 



0.4 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



w 



403 



6,780 



0.5 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



s 



403 



6,780 



0.1 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



w 



751 



5,640 



0.5 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



s 



751 



5,640 



0.3 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



w 



1,064 



5,300 



0.3 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



s 



1,064 



5,300 



0.4 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



w 



197 



2,340 



0.6 



u 



INCO (3) 



Ni-Vee Bronze B 



- 



s 



197 



2,340 



<0.1 



NU-ET 



INCO (3) 



Ni-Vee Bronze B 



- 



w 



402 



2,370 



1.2 



U 



INCO (3) 



Ni-Vee Bronze B 



- 



s 



402 



2,370 



<0.1 



ET 



INCO (3) 



Ni-Vee Bronze B 



- 



w 



181 



5 



1.8 



P(4) 



INCO (3) 



Ni-Vee Bronze B 



- 



w 



366 



5 



1.3 



CR(6) 



INCO (3) 



Ni-Vee Bronze C e 



- 



w 



123 



5,640 



0.8 



U 



INCO (3) 



Ni-Vee Bronze C 



- 



s 



123 



5,640 



0.5 



U 



INCO (3) 



Ni-Vee Bronze C 



- 



w 



403 



6,780 



0.8 



U 



INCO (3) 



Ni-Vee Bronze C 



- 



s 



403 



6,780 



0.2 



U 



INCO (3) 



Ni-Vee Bronze C 



- 



w 



751 



5,640 



2.0 



G 



INCO (3) 



76 



